- Nano Express
- Open Access
Modified microwave method for the synthesis of visible light-responsive TiO2/MWCNTs nanocatalysts
© Alosfur et al.; licensee Springer. 2013
- Received: 16 May 2013
- Accepted: 23 July 2013
- Published: 6 August 2013
Recently, TiO2/multi-walled carbon nanotube (MWCNT) hybrid nanocatalysts have been a subject of high interest due to their excellent structures, large surface areas and peculiar optical properties, which enhance their photocatalytic performance. In this work, a modified microwave technique was used to rapidly synthesise a TiO2/MWCNT nanocatalyst with a large surface area. X-ray powder diffraction, field-emission scanning electron microscopy, transmission electron microscopy and Brunauer-Emmett-Teller measurements were used to characterise the structure, morphology and the surface area of the sample. The photocatalytic activity of the hybrid nanocatalysts was evaluated through a comparison of the degradation of methylene blue dye under irradiation with ultraviolet and visible light. The results showed that the TiO2/MWCNT hybrid nanocatalysts degraded 34.9% of the methylene blue (MB) under irradiation with ultraviolet light, whereas 96.3% of the MB was degraded under irradiation with visible light.
- Hybrid nanocatalysts
Industrial advancements over the past several decades have led to an upsurge in the rate of water consumption. Due to the scarcity of clean water resources, the recycling of water via the elimination of extremely coloured wastewater has become important. Different methods, such as adsorption , oxidation , reduction  and anaerobic treatments , have been developed for the elimination of dyes from effluents. Unfortunately, these methods have several disadvantages [5–7], which have triggered interest among scientists in developing a method to decompose the undesirable organic compounds, such as dyes, via photocatalytic processes using the semiconductor degradation method [8–10]. This method offers several advantages, such as being simpler, cheaper and cleaner. Hence, this method is acknowledged as being a ‘greener’ technology for the elimination of toxic organic and inorganic pollutants from wastewater at ambient temperature and pressure [11–13].
Titania (TiO2) nanoparticles have been identified as a suitable material for the removal of dyes from effluents. However, due to its wide bandgap (3.2 eV), TiO2 exhibits photocatalytic activation only under UV irradiation (λ ≤ 384 nm), which accounts for only 7% of the total solar energy . Several methods have been suggested to improve the photocatalytic activity of TiO2 in the visible light range [15–17]. Unfortunately, these methods involve compounds that are either thermally unstable, difficult to modify or even toxic .
Recently, there is growing interest in the hybridisation of TiO2 and carbon-based nanostructures, namely single-walled carbon nanotubes (SWCNTs) [19, 20], multi-walled carbon nanotubes (MWCNT) [21, 22] and graphene [23, 24], as an attempt to improve the photocatalytic activity of TiO2. This improvement was attributed to three main factors namely the enlarged absorption region of TiO2[25–27], enhanced electronic transfer and thus reduced electron accumulation in TiO2 nanoparticles [28, 29] and extremely high surface area [30, 31].
The TiO2 nanoparticle attachment to MWCNTs can be prepared using different methods, such as hydrothermal , sol-gel  or electrochemical  methods. However, most of these methods require long preparation times (several hours or a day), involve multiple steps and have high thermal costs, which often result in structural damage in the MWCNTs. Thus, there is a need to develop an easier and faster method for their synthesis.
The synthesis of nanostructured materials via microwave irradiation has been reported to be an effective technique [34–36]. This technique offers several advantages, such as simple and fast synthesis procedures, improved reaction kinetics, uniform heat distribution and minimal structural damage . In this work, a novel technology is presented for the synthesis of a hybrid photocatalytic material with greater photocatalytic activities and a wider spectral response range using a modified microwave method. Our previous report detailed the synthesis and optical properties of TiO2/MWCNTs hybrid nanocatalysts using a modified microwave method . The results showed an enhancement in the optical absorbance, which was shifted from the UV to the visible light region after the MWCNTs were decorated with TiO2 nanoparticles. Here, we demonstrate our extended effort to extensively study the structural properties and, in particular, the photocatalytic application of these hybrid nanocatalysts.
A modified microwave method was used to synthesise the TiO2/MWCNTs hybrid nanocatalysts. Initially, a 3.5-cm hole was drilled through the top of a household microwave oven. A reflux condenser was subsequently installed in the microwave oven to enable continuous synthesis at ambient pressures. Since the microwave has a wavelength of 12 cm, there will be no escaped radiation through the hole. As additional protection purpose, the microwave was operated inside a fume hood. Commercial MWCNTs (Cheap Tubes Inc., Brattleboro, VT, USA) with an outer diameter of 10 to 30 nm, an inner diameter of 5 nm, a surface area of 110 m2/g and lengths up to 50 μm were used in this work. Due to electrostatic interactions and van der Waals forces between the individual nanotubes, the MWCNTs exhibit a strong tendency to agglomerate. This agglomeration leads to poor solubility of the MWCNTs in most aqueous and organic solvents. Thus, to achieve a stable aqueous suspension of MWCNTs, functionalisation processes are necessary due to the presence of a large amount of functional groups on the nanotubes' surface. The presence of these functional groups on the MWCNTs' surface imparts negative charges and thus generates repulsion forces, which inhibit agglomeration. These negative charges can also function as anchor sites and thereby enable the in situ attachment of synthesised nanoparticles onto the MWCNTs' surface.
For this purpose, the MWCNTs were first functionalised by being sonicated for 3 h in a 65% solution of concentrated HNO3. The suspended MWCNTs were then placed in the modified microwave oven (Sharp model R-369 T) and irradiated for 20 min at a power of 550 W. Afterwards, the product was rinsed with deionised water six times and then completely dried at 80°C. The MWCNTs were denoted as functionalised MWCNTs (f-MWCNTs) after this process. The surface areas of the f-MWCNTs dramatically increased to 357.6 m2/g after the functionalisation process. Greater MWCNT surface area recorded after functionalisation has been associated with the increase of functional groups on the nanotube surface .
Preparation of TiO2/MWCNTs nanocatalysts involved the dispersion of f-MWCNTs in ethanol (pH = 2) and sonicated for 1 h. Then, approximately 561 μL of titanium isopropoxide (TTIP) was added dropwise to the suspension over a period of 20 min under vigorous stirring. Notably, under acidic conditions, the TiO2 surface contains positive charges due to the presence of ≡Ti-OH2+ groups , which enhance the adhesion characteristics on the MWCNTs' surface.
The amount of TTIP precursor represented a TiO2/f-MWCNT weight ratio of 50%. The mixture was then placed inside the modified microwave oven and irradiated for 5 min at a power of 550 W under continuous stirring. This suspension was subsequently dried at 100°C in a drying oven and then calcined at 500°C in air for 1 h to prepare the hybrid nanocatalysts.
The crystalline structure of the TiO2/MWCNTs nanocatalyst was characterised using X-ray powder diffraction (XRD) (Bruker D8 Advance, Karlsruhe, Germany) equipped with a Cu Kα radiation source operated at 40 kV and 40 mA. The powder morphology was determined by field-emission scanning electron microscopy (FE-SEM; SUPRA 55VP, Carl Zeiss, Jena, Germany) and transmission electron microscopy (TEM; Philips CM12, Amsterdam, The Netherlands; operated at 80 kV) studies. In addition, a Brunauer-Emmett-Teller (BET) (Micromeritics, ASAP 2020, Georgia, USA) was used to determine the surface area of the nanocatalyst.
The photocatalytic activity of the TiO2/MWCNTs nanocatalyst was evaluated by monitoring the degradation of methylene blue (MB) in an aqueous solution under irradiation with ultraviolet (UV) (VL-6.LC lamp) or visible light (VL) (commercial halogen tungsten lamp) using a custom-built setup. A small amount (1 mg) of the sample was suspended in 100 ml of aqueous MB solution with a concentration of 10 ppm. Prior to illumination, the solution was sonicated for 10 min and placed in a dark room for 1 h, thus permitting equilibration of the adsorption–desorption of the dye on the nanocatalyst surface. The first sample (approximately 5 mL) solution was collected immediately and was taken as the initial MB concentration (c0). The solution was then continuously shaken at 200 rpm. Approximately 5 mL of the liquid was withdrawn every 20 min and immediately centrifuged to remove any suspended solids. To monitor the degradation of the MB, the clean solution was then analysed using a UV–Visible spectrometer (Perkin Elmer, Lambda 900 UV/Vis) in the range of 500–750 nm.
At low pressures, the surface is only partially occupied by the gas, whereas the monolayer is filled and the isotherm reaches a plateau at higher pressures. Based on these results, the nanocatalyst can be ascribed to a type IV adsorption isotherm according to the IUPAC classification scheme; this result suggests that the structure of the nanocatalyst is mesoporous.
The pore size distribution of the TiO2/MWCNTs nanocatalysts was investigated based on the Barrett-Joyner-Halenda process (inset in Figure 4). The material shows bimodal mesopore size distributions, i.e. narrow mesopores with peak pore diameters of approximately 2.5 nm and larger mesopores with peak pore diameters of approximately 3.4 nm .
We successfully synthesised a hybrid nanocatalyst by attaching TiO2 nanoparticles onto MWCNTs at a weight ratio of 50% using a novel one-step method. The microstructure and morphology of the hybrid nanocatalyst were characterised by XRD, FESEM and TEM. The results showed that the anatase-phase TiO2 nanoparticles were attached to the surface of the MWCNTs. The BET surface area of the MWCNTs decreased after the TiO2 was attached to their surface. In addition, the efficiency of MB degradation under visible light was substantially greater compared to the efficiency under ultraviolet irradiation. These results indicate that MWCNTs can act as a photosensitiser agent and are excited under visible-light irradiation.
The authors would like to thank Universiti Kebangsaan Malaysia for providing the financial support for this work through DIP-2012-32 and DPP-2013-048 research grants.
- Murugan K, Rao TN, Gandhi AS, Murty B: Effect of aggregation of methylene blue dye on TiO2 surface in self-cleaning studies. Catal Commun 2010, 11: 518–521. 10.1016/j.catcom.2009.12.007View ArticleGoogle Scholar
- Schäfer A, Nghiem L, Waite T: Removal of the natural hormone estrone from aqueous solutions using nanofiltration and reverse osmosis. Environ Sci Technol 2003, 37: 182–188. 10.1021/es0102336View ArticleGoogle Scholar
- Zhang M, Wang J, Fu H: Preparation and photocatalytic activity of nanocrystalline TiO2 with uniform shape and size. J Mater Process Technol 2008, 199: 274–278. 10.1016/j.jmatprotec.2007.08.037View ArticleGoogle Scholar
- Yasar A, Tabinda AB: Anaerobic treatment of industrial wastewater by UASB reactor integrated with chemical oxidation processes; an overview. Pol J Environ Stud S 2010, 19: 1051–1061.Google Scholar
- Malato S, Fernández-Ibáñez P, Maldonado M, Blanco J, Gernjak W: Decontamination and disinfection of water by solar photocatalysis: recent overview and trends. Catal Today 2009, 147: 1–59. 10.1016/j.cattod.2009.06.018View ArticleGoogle Scholar
- Chaudhari K, Bhatt V, Bhargava A, Seshadri S: Combinational system for the treatment of textile waste water: a future perspective. Asian J Water Environ Pollut 2011, 8: 127–136.Google Scholar
- Hai FI, Yamamoto K, Fukushi K: Hybrid treatment systems for dye wastewater. Crit Rev Env Sci Technol 2007, 37: 315–377. 10.1080/10643380601174723View ArticleGoogle Scholar
- Rauf M, Meetani M, Hisaindee S: An overview on the photocatalytic degradation of azo dyes in the presence of TiO2 doped with selective transition metals. Desalination 2011, 276: 13–27. 10.1016/j.desal.2011.03.071View ArticleGoogle Scholar
- Akpan U, Hameed B: Parameters affecting the photocatalytic degradation of dyes using TiO2-based photocatalysts: a review. J Hazard Mater 2009, 170: 520–529. 10.1016/j.jhazmat.2009.05.039View ArticleGoogle Scholar
- Toor AP, Verma A, Jotshi C, Bajpai P, Singh V: Photocatalytic degradation of direct yellow 12 dye using UV/TiO2 in a shallow pond slurry reactor. Dyes Pigm 2006, 68: 53–60. 10.1016/j.dyepig.2004.12.009View ArticleGoogle Scholar
- Liu K, Zhu L, Jiang T, Sun Y, Li H, Wang D: Mesoporous TiO2 micro-nanometer composite structure: synthesis, optoelectric properties, and photocatalytic selectivity. Int J Photoenergy 2012, 2012: 1–14.Google Scholar
- Robert D, Malato S: Solar photocatalysis: a clean process for water detoxification. Sci Total Environ 2002, 291: 85–97. 10.1016/S0048-9697(01)01094-4View ArticleGoogle Scholar
- Gaya UI, Abdullah AH: Heterogeneous photocatalytic degradation of organic contaminants over titanium dioxide: a review of fundamentals, progress and problems. J Photochem Photobiol, C 2008, 9: 1–12. 10.1016/j.jphotochemrev.2007.12.003View ArticleGoogle Scholar
- Hernández-Alonso MD, Fresno F, Suárez S, Coronado JM: Development of alternative photocatalysts to TiO2: challenges and opportunities. Energy Environ Sci 2009, 2: 1231–1257. 10.1039/b907933eView ArticleGoogle Scholar
- Xiang Q, Yu J, Jaroniec M: Nitrogen and sulfur co-doped TiO2 nanosheets with exposed 001 facets: synthesis, characterization and visible-light photocatalytic activity. Phys Chem Chem Phys 2011, 13: 4853–4861. 10.1039/c0cp01459aView ArticleGoogle Scholar
- Yu H, Irie H, Shimodaira Y, Hosogi Y, Kuroda Y, Miyauchi M, Hashimoto K: An efficient visible-light-sensitive Fe (III)-grafted TiO2 photocatalyst. J Phys Chem C 2010, 114: 16481–16487. 10.1021/jp1071956View ArticleGoogle Scholar
- Yao W, Zhang B, Huang C, Ma C, Song X, Xu Q: Synthesis and characterization of high efficiency and stable Ag3PO4/TiO2 visible light photocatalyst for the degradation of methylene blue and rhodamine B solutions. J Mater Chem 2012, 22: 4050–4055. 10.1039/c2jm14410gView ArticleGoogle Scholar
- Hashimoto K, Irie H, Fujishima A: TiO2 photocatalysis: a historical overview and future prospects. AAPPS Bull 2007, 17: 8269–8285.Google Scholar
- Zhou W, Pan K, Qu Y, Sun F, Tian C, Ren Z, Tian G, Fu H: Photodegradation of organic contamination in wastewaters by bonding TiO2/single-walled carbon nanotube composites with enhanced photocatalytic activity. Chemosphere 2010, 81: 555–561. 10.1016/j.chemosphere.2010.08.059View ArticleGoogle Scholar
- Clemens P, Wei X, Wilson BL, Thomas RL: Anatase titanium dioxide coated single wall carbon nanotubes manufactured by sonochemical-hydrothermal. Jour Compos Mater 2013, 3: 21–32.Google Scholar
- Vatanpour V, Madaeni SS, Moradian R, Zinadini S, Astinchap B: Novel antibifouling nanofiltration polyethersulfone membrane fabricated from embedding TiO2 coated multiwalled carbon nanotubes. Sep Purif Technol 2012, 90: 69–82.View ArticleGoogle Scholar
- Zhao D, Yang X, Chen C, Wang X: Enhanced photocatalytic degradation of methylene blue on multiwalled carbon nanotubes-TiO2. J Colloid Interface Sci 2013, 111: 1–6.Google Scholar
- Min Y, Zhang K, Zhao W, Zheng F, Chen Y, Zhang Y: Enhanced chemical interaction between TiO2 and graphene oxide for photocatalytic decolorization of methylene blue. Chem Eng J 2012, 193: 203–210.View ArticleGoogle Scholar
- Zhao D, Sheng G, Chen C, Wang X: Enhanced photocatalytic degradation of methylene blue under visible irradiation on graphene@TiO2 dyade structure. Appl Catal, B 2012, 111: 303–308.View ArticleGoogle Scholar
- Zhang Q, Li C, Li T: Rapid photocatalytic degradation of methylene blue under high photon flux UV irradiation: characteristics and comparison with routine low photon flux. Int J Photoenergy 2012, 2012: 1–7.Google Scholar
- Liu J, An T, Li G, Bao N, Sheng G, Fu J: Preparation and characterization of highly active mesoporous TiO2 photocatalysts by hydrothermal synthesis under weak acid conditions. Microporous Mesoporous Mater 2009, 124: 197–203. 10.1016/j.micromeso.2009.05.009View ArticleGoogle Scholar
- Réti B, Németh K, Németh Z, Mogyorósi K, Markó K, Erdőhelyi A, Dombi A, Hernadi K: Photocatalytic measurements of TiO2/MWCNT catalysts having different surface coverage. Phys Status Solidi B 2011, 248: 2475–2479. 10.1002/pssb.201100080View ArticleGoogle Scholar
- Zhang K, MENG Z, OH W: Degradation of rhodamine B by Fe-carbon nanotubes/TiO2 composites under UV light in aerated solution. Chin J Catal 2010, 31: 751–758. 10.1016/S1872-2067(09)60084-XView ArticleGoogle Scholar
- Hu C, Zhang R, Xiang J, Liu T, Li W, Li M, Duo S, Wei F: Synthesis of carbon nanotube/anatase titania composites by a combination of sol–gel and self-assembly at low temperature. J Solid State Chem 2011, 184: 1286–1292. 10.1016/j.jssc.2011.03.040View ArticleGoogle Scholar
- Xie Y, Qian H, Zhong Y, Guo H, Hu Y: Facile low-temperature synthesis of carbon nanotube/TiO2 nanohybrids with enhanced visible-light-driven photocatalytic activity. Int J Photoenergy 2012, 2012: 1–6.View ArticleGoogle Scholar
- Li Z, Gao B, Chen GZ, Mokaya R, Sotiropoulos S, Li Puma G: Carbon nanotube/titanium dioxide (CNT/TiO2) core–shell nanocomposites with tailored shell thickness, CNT content and photocatalytic/photoelectrocatalytic properties. Appl Catal, B 2011, 110: 50–57.View ArticleGoogle Scholar
- Yang H, Wu S, Duan Y, Fu X, Wu J: Surface modification of CNTs and enhanced photocatalytic activity of TiO2 coated on hydrophilically modified CNTs. Appl Surf Sci 2012, 258: 3012–3018. 10.1016/j.apsusc.2011.11.029View ArticleGoogle Scholar
- Wang GJ, Lee MW, Chen YH: A TiO2/CNT coaxial structure and standing CNT array laminated photocatalyst to enhance the photolysis efficiency of TiO2. Photochem Photobiol 2008, 84: 1493–1499. 10.1111/j.1751-1097.2008.00374.xView ArticleGoogle Scholar
- Mahmood MA, Dutta J: Microwave assisted hydrothermal synthesis of zinc hydroxystannate films on glass substrates. J Sol-gel Sci Technol 2012, 62: 495–504. 10.1007/s10971-012-2754-2View ArticleGoogle Scholar
- Caddick S, Fitzmaurice R: Microwave enhanced synthesis. Tetrahedron 2009, 65: 3325–3355. 10.1016/j.tet.2009.01.105View ArticleGoogle Scholar
- He Z, Yang S, Ju Y, Sun C: Microwave photocatalytic degradation of rhodamine B using TiO2 supported on activated carbon: mechanism implication. J Environ Sci 2009, 21: 268–272. 10.1016/S1001-0742(08)62262-7View ArticleGoogle Scholar
- Cui L, Hui K, Hui K, Lee S, Zhou W, Wan Z, Thuc CNH: Facile microwave-assisted hydrothermal synthesis of TiO2 nanotubes. Mater Lett 2012, 75: 175–178.View ArticleGoogle Scholar
- Jumali MHH, Alosfur F, Radiman S, Umar AA: Dressing of MWCNTs with TiO2 nanoparticles using modified microwave method. Adv Mat Res 2012, 364: 228–231.Google Scholar
- Carabineiro SA, Pereira MF, Pereira JN, Caparros C, Sencadas V, Lanceros-Mendez S: Effect of the carbon nanotube surface characteristics on the conductivity and dielectric constant of carbon nanotube/poly (vinylidene fluoride) composites. Nanoscale Res Lett 2011, 6: 1–5.Google Scholar
- Choi W: Pure and modified TiO2 photocatalysts and their environmental applications. Catal Surv Asia 2006, 10: 16–28. 10.1007/s10563-006-9000-2View ArticleGoogle Scholar
- Zaine SNA, Mastan AAK, Shaik Ahmedullah S, Mohamed NM, Ramli A, Ahmad IA: Synthesis and characterization of pure anatase TiO2 aggregates. J Appl Sci 2011, 11: 1326–1330.View ArticleGoogle Scholar
- Sánchez M, Guirado R, Rincón M: Multiwalled carbon nanotubes embedded in sol–gel derived TiO2 matrices and their use as room temperature gas sensors. J Mater Sci Mater Electron 2007, 18: 1131–1136. 10.1007/s10854-007-9144-5View ArticleGoogle Scholar
- Rakhi R, Sethupathi K, Ramaprabhu S: Field emission properties of metal encapsulated and metal-oxide dispersed multi-walled carbon nanotube nanocomposites. J Nano Energy Power Res 2011, 1: 57–64. 10.1166/jnepr.2011.1008View ArticleGoogle Scholar
- Yu J, Ma T, Liu S: Enhanced photocatalytic activity of mesoporous TiO2 aggregates by embedding carbon nanotubes as electron-transfer channel. Phys Chem Chem Phys 2010, 13: 3491–3501.View ArticleGoogle Scholar
- Németh Z, Dieker C, Kukovecz Á, Alexander D, Forró L, Seo JW, Hernadi K: Preparation of homogeneous titania coating on the surface of MWNT. Compos Sci Technol 2011, 71: 87–94. 10.1016/j.compscitech.2010.10.017View ArticleGoogle Scholar
- Chen L, Pang X, Yu G, Zhang J: In-situ coating of MWNTs with sol–gel TiO2 nanoparticles. Adv Mater Lett 2010, 1: 75–78. 10.5185/amlett.2010.4117View ArticleGoogle Scholar
- Zhang K, Zhang FJ, Chen ML, Oh WC: Comparison of catalytic activities for photocatalytic and sonocatalytic degradation of methylene blue in present of anatase TiO2–CNT catalysts. Ultrason Sonochem 2011, 18: 765–772. 10.1016/j.ultsonch.2010.11.008View ArticleGoogle Scholar
- Song C, Chen P, Wang C, Zhu L: Photodegradation of perfluorooctanoic acid by synthesized TiO2–MWCNT composites under 365 nm UV irradiation. Chemosphere 2012, 86: 853–859. 10.1016/j.chemosphere.2011.11.034View ArticleGoogle Scholar
- Yu J, Fan J, Cheng B: Dye-sensitized solar cells based on anatase TiO2 hollow spheres/carbon nanotube composite films. J Power Sources 2011, 196: 7891–7898. 10.1016/j.jpowsour.2011.05.014View ArticleGoogle Scholar
- Woan K, Pyrgiotakis G, Sigmund W: Photocatalytic carbon-nanotube–TiO2 composites. Adv Mater 2009, 21: 2233–2239. 10.1002/adma.200802738View ArticleGoogle Scholar
- Huang HC, Huang GL, Chen HL, Lee YD: Immobilization of TiO2 nanoparticles on carbon nanocapsules for photovoltaic applications. Thin Solid Films 2006, 511: 203–207.View ArticleGoogle Scholar
- Lu SY, Tang CW, Lin YH, Kuo HF, Lai YC, Tsai MY, Ouyang H, Hsu WK: TiO2-coated carbon nanotubes: a redshift enhanced photocatalysis at visible light. Appl Phys Lett 2010, 96: 231915–231913. 10.1063/1.3454908View ArticleGoogle Scholar
- Jiang G, Zheng X, Wang Y, Li T, Sun X: Photo-degradation of methylene blue by multi-walled carbon nanotubes/TiO2 composites. Powder Technol 2011, 207: 465–469. 10.1016/j.powtec.2010.11.029View ArticleGoogle Scholar
- Tian L, Ye L, Deng K, Zan L: TiO2/carbon nanotube hybrid nanostructures: solvothermal synthesis and their visible light photocatalytic activity. J Solid State Chem 2011, 184: 1465–1471. 10.1016/j.jssc.2011.04.014View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.